Cryogenics 54 (2013) 44–49
Contents lists available at SciVerse ScienceDirect
Cryogenics journal homepage: www.elsevier.com/locate/cryogenics
Apparatus for calorimetric measurements of losses in MgB2 superconductors exposed to alternating currents and external magnetic ﬁelds H. Taxt a,1, N. Magnusson b,⇑, M. Runde a,b a b
Department of Electrical Power Engineering, Norwegian University of Science and Technology, NO-7491 Trondheim, Norway SINTEF Energy Research, NO-7465 Trondheim, Norway
a r t i c l e
i n f o
Article history: Received 24 August 2012 Received in revised form 15 January 2013 Accepted 26 January 2013 Available online 8 February 2013 Keywords: AC losses Calorimetric measurements MgB2 Superconductors
a b s t r a c t Inexpensive superconducting wires with low AC losses would open up for a large superconductor market in AC electrical power applications. One candidate for this market is the MgB2 conductor. In the development of an AC optimized superconductor, high-quality measurements of the AC losses under applicationlike conditions must be available. This article describes an apparatus built for this purpose. The measurement method is calorimetric. The temperature increase of the superconductor sample is measured and compared to the temperature increase due to a heater with known heat input. The system is designed for measurements of losses due to magnetic ﬁelds combined with transport currents. Results from tests verifying the capabilities of the system are given, as well as from initial AC loss measurements on a tapeshaped MgB2 superconductor. Ó 2013 Elsevier Ltd. All rights reserved.
1. Introduction Superconductors have for decades been acknowledged as materials that could introduce major beneﬁts to electric power systems. The possibility to reduce losses and dramatically increase current densities would push the limits of traditional electric power components, such as transformers, cables and motors. However, still the commercial applications are few and the potential of the materials unutilized. One issue to be solved for a broad use of superconductors in AC applications is the reduction of AC losses. In the late 1980s, intensive efforts were put into the reduction of the AC losses in BSSCO/ Ag superconductors. The results did not lead to a commercial breakthrough. More recently, the MgB2 superconductor has been developed into long-length wires. This conductor is inexpensive and more easily manufactured, with prospects of a successful AC loss reduction . AC losses inevitably appear when a superconductor is exposed to an AC magnetic ﬁeld (externally applied or generated by a transport current), due to the irreversible motion of vortices pushed in and out of the superconductor every half cycle, resulting in hysteresis losses. The AC losses, Pac, are for a given conductor a function of temperature, T, magnetic ﬁeld, B, transport current, I, and frequency, f,
⇑ Corresponding author. Tel.: +47 73597269; fax: +47 73597250. 1
E-mail address: [email protected]
(N. Magnusson). Present address: SINTEF Energy Research, NO-7465 Trondheim, Norway.
0011-2275/$ - see front matter Ó 2013 Elsevier Ltd. All rights reserved. http://dx.doi.org/10.1016/j.cryogenics.2013.01.002
Pac ¼ Pac ðT; B; I; f Þ:
High quality measurements of AC losses are necessary for the development of good AC superconductors. Two different principles for measuring the losses in superconductors (both used extensively for BSCCO/Ag tapes) dominate in the literature, the electromagnetic [2,3] and the calorimetric [4–6], with good agreement of the results of the two methods . The electromagnetic method is generally faster, and for BSCCO/Ag tapes it requires less thermal considerations as the sample simply can be immersed in liquid nitrogen. On the other hand, the calorimetric method involves less complicated electrical measurements and directly yields the total loss. For MgB2 superconductors, measurements of the losses due to AC magnetic ﬁelds [8,9], due to transport currents , and by combinations of a DC magnetic ﬁeld and transport currents  have been reported. The apparatus presented in this article enables loss measurements in any combination of magnetic ﬁelds and transport currents, AC or DC, simulating the likely conditions in AC power components. The measurement system is calorimetric. For measurements in the 20–40 K range, in contrast to the case at 77 K, conduction cooling and vacuum need to be introduced and consequently adds no further complication compared to the electromagnetic method. The system’s design is based on a previous system for BSCCO/Ag tapes reported in [4,11], but aims for the MgB2 application range. That is, temperatures down to 20 K and magnetic ﬁelds up to 1 T (peak) and transport currents of several hundred amperes should be handled. The principle of the measurement method is explained in Section 2, an overview of the system and detailed descriptions of
H. Taxt et al. / Cryogenics 54 (2013) 44–49
key parts are given in Section 3. In Section 4 results from system veriﬁcation measurements and ﬁnally initial AC loss measurements on an MgB2 wire are given. 2. Measurement principle In the calorimetric method, we measure the temperature increase of the superconducting sample when exposed to an AC magnetic ﬁeld and/or a transport current. In principle, for an adiabatic system the power loss is given by,
Pac ¼ C DT ac =Dt ac ;
where C is the heat capacity, DTac the temperature increase and, Dtac the measurement time. However, C is not known and the system is not fully adiabatic. Therefore, the system is calibrated by measuring the temperature increase due to a known heat input in a heater wound together with the sample. The heat capacity is then eliminated from (2) and the power loss is given by,
Pac ¼ ðDT AC Dt cal =DT cal DtAC ÞPcal ;
where DTcal is the temperature increase during calibration, Dtcal the calibration time, and Pcal the power input during calibration. Note that (3) only holds for an adiabatic system. Therefore, the durations, Dtac and Dtcal, should be kept equal. To account also for the heat transmitted from the sample and the change in heat capacity with temperature, a calibration ratio, rc, can be introduced,
r c ðDtcal ; TÞ ¼ ðDt cal =DT cal ÞPcal
O-ring at ambient temperature. Between the upper and lower cryostat parts, an evacuable space is formed, where a sample holder and the sample are placed and can be cooled down to the desired temperatures by a cooling machine. A set of thermal radiation shields and the use of liquid nitrogen on the outside of parts of the cryostat reduce the thermal load to the cooling machine. The sample is arranged in a ring enabling magnetic ﬁeld generation by circular ﬁeld coils. The sample length is chosen long enough to meet the requirements of minimal bending radius for most samples and to ensure a measurement length with uniform temperature, and it is chosen short enough to enable the generation of a strong magnetic ﬁeld (low enough inductance in the coils) and for sample preparation practicability. A cross-section overview of the measurement system is shown in Fig. 1 and a photo of the lower part of the system in Fig. 2. The system is cylindrically symmetric. The sample (1) is placed in the form of a ring, with a diameter of 0.28 m, on top of a sample holder (2), which is in thermal contact with the cold head of a cooling machine (3). These parts are situated in vacuum enclosed by a cryostat (4). The reservoir (5) at the top is ﬁlled with liquid nitrogen to limit the heat radiation. At the side (6) and at the bottom (7) radiation shields covered with superinsulation are inserted inside the vacuum to limit the heat radiation in these regions. The latter shield is cooled by liquid nitrogen from outside the cryostat. For magnetic ﬁeld generation, copper coils (8) are placed in the liquid nitrogen reservoir on both sides of the sample. Transport currents are injected at the bottom of the cryostat through a
During calibration, the function rc(Dtcal, T) is determined for relevant measurement durations and loss levels, see Section 4. 3. Measurement system design 3.1. System overview Several different aspects need to be considered to realize a measurement system with the desired operating ranges and measurement sensitivity. The low measurement temperature and the high magnetic ﬁelds and transport currents involved impose constraints on the design and material choices. The cryostat is built of ﬁbreglass reinforced epoxy tubes and plates which are glued together. This material is strong, sustains low temperatures, has a thermal contraction comparable to that of metals, and is non-conducting (avoiding induced currents). To allow for sample preparation, the cryostat is divided in a lower and an upper part sealed with an
Fig. 2. Figure of the lower part of the cryostat and the sample holder with the sample.
Fig. 1. Cross-sectional view of the apparatus. The system is cylindrically symmetric around the centre axis.
H. Taxt et al. / Cryogenics 54 (2013) 44–49
copper current feed through (9), cooled by liquid nitrogen on the outside, and then transported via a BSSCO/Ag conductor to a wire cooler (10), where the BSCCO/Ag conductor is soldered to the MgB2 sample conductor (not part of the 2D ﬁgure). Measurement wires are inserted through a separate signal feed through (11). 3.2. Sample arrangement The sample is glued to the sample holder using Stycast 2850, ensuring good thermal contact. In Fig. 3 arrangements for round and for tape shaped samples are shown. A high-ohmic wire (80 X/m) used as heater is wound together with the samples, twisted around the round sample and simply attached to the outside of the tape shaped sample. Similarly a copper wire is wound biﬁlarly along half of the sample length (to the far side from the point of current injection). The copper wire is used as thermometer (in the 20–40 K range the change in resistance is signiﬁcant for copper) and measures the temperature increase during AC loss measurements and calibration. The copper thermometers were approximately 1 m long and carried currents of 100 mA. At the measurement temperatures the power in the thermometers was around 0.3 mW. Tests were performed by reducing the current input to the copper thermometer to 50 mA, showing no notable change in measured resistance, and hence temperature, assuring that the measurement current did not inﬂuence the temperature measurements. It is important that the temperature is uniform over the half-turn, and therefore, to control the uniformity, additional shorter copper thermometers are attached at different positions along the sample. The copper thermometers are calibrated in advance with a Cernox temperature sensor. 3.3. Thermal properties close to the sample The sample holder is made of a 3 mm thick glass-ﬁbre reinforced epoxy tube, with a 0.5 mm thick copper plate (thermally connected to the cold head) glued to the outside, see Fig. 4. The choice of thermal resistance between the sample and the cold head (and consequently in this case the copper plate), is a trade-off between achievable temperature and cool-down time on one side, and measurement sensitivity on the other. A 20 mm space between the copper plate (divided into teeth to avoid large induced currents during AC magnetic ﬁeld exposure) and the sample results in a thermal resistance of about 30 K/W at 25 K, high enough to see a distinct temperature increase in the sample, and low enough to allow for cooling down within a reasonable time (a few hours). To enable variation of the sample temperature without introducing large power inputs directly to the sample, a second heater is glued to the top of the sample holder. By adjusting the power
Fig. 4. Top of sample holder.
dissipated in this wire between 0 and 1 W, sample temperatures in the range 20–50 K can be obtained. 3.4. Insulation and cooling system The sample is placed in vacuum, enclosed by a cryostat, which is built of ﬁbre-glass reinforced epoxy to avoid inducing electrical currents and heat dissipation. A pressure of the order 102 mbar is obtained with a vacuum pump before turning on the cooling machine, and a pressure below 103 mbar is obtained when the cold head acts as a cold trap. At this latter pressure, heat is transferred mainly by radiation. At the top of the cryostat, the radiation is limited by ﬁlling the reservoir with liquid nitrogen. At the lower side, a radiation shield, covered with superinsulation and thermally anchored to liquid nitrogen on the outside of the cryostat, withdraws heat radiated from the bottom cryostat wall. An additional radiation shield with superinsulation faces the outer cylinder wall to avoid frost on the outside of that wall. The measurement wires (copper thermometers and voltage taps) which enter the vacuum space at room temperature, are ﬁrst thermally anchored to the lower radiation shield at about 77 K, and then thermally anchored to a wire cooler (not shown in Fig. 1) at about 20 K before entering the sample. With these arrangements, the total thermal load to the cooling machine is only a few watts. 3.5. Magnetizing coils The magnetic ﬁeld that the sample is exposed to is generated by passing current in a pair of copper coils concentric with the sample and placed in the liquid nitrogen bath, close to the sample (see
Fig. 3. Sketch of the sample arrangement with round and tape shaped samples. The heater and the copper thermometer are glued to the sample using Stycast 2850.
H. Taxt et al. / Cryogenics 54 (2013) 44–49
Fig. 1). The inner and outer coils are connected in antiparallel, with the main purpose of the inner coil to reduce the inductance of the coil pair. Each coil consists of 44 turns of a 2 mm 12.5 mm vanish insulated copper strand, ﬁlling a coil cross-section area of 25 mm 50 mm. The magnetic ﬁeld generated over the sample is 0.62 mT per ampere in the coils. At the sample location, the magnetic ﬁeld is vertically directed. For round samples the direction of the magnetic ﬁeld in the plane perpendicular to the current path is unimportant. However, for rectangular or tape-shaped samples one may want to vary the magnetic ﬁeld direction in this plane. This can be done e.g. by passing currents in only the outer coil and step-wise moving it upwards and thereby change the magnetic ﬁeld orientation over the sample. Since the coils are immersed in liquid nitrogen, large currents can be allowed, particularly for short periods of time. At a current of 1.14 kArms the magnetic ﬁeld over the sample is 1 Tpeak. This current, corresponding to a current density of 44 A/mm2, results in a temperature increase (assuming adiabatic conditions) in the copper coil of about 20 K after 3 s, a time sufﬁcient for making an AC loss measurement in high magnetic ﬁelds (at which the losses are expected to be the highest). The resistance of the coils is about 0.01 X and the inductance 0.7 mH. At 50 Hz the inductance dominates the impedance (0.2 X). To reduce reactive power requirements from the power source, capacitive compensation is used, reducing the impedance of the circuit and enabling experiments to be carried out in a standard laboratory. One should note, though, that when applying a controlled AC voltage to the coils, the circuit should not be fully compensated, as heating of the coils causes their resistance to increase, thereby also changing the current. The AC loss measurements presented in Section 4.2 demonstrate magnetic ﬁelds up to 0.1 T, whereas subsequent measurements  have been performed up to 0.3 T. Higher ﬁelds have so far not been demonstrated, but may be of interest if and when low AC loss MgB2 wires become available.
For measurements with transport currents only, the current can be supplied directly from a power source. For combinations of magnetic ﬁelds and transport currents, a current transformer is used to keep the magnetic ﬁeld and sample current in-phase. The magnetic ﬁeld coils are then connected in series with the primary winding of the transformer, whereas the sample current is fed from the secondary winding. The ratio between magnetic ﬁeld and transport current is varied by changing the ratio between the turns of the transformer windings. 4. Veriﬁcation and loss measurements 4.1. System veriﬁcation and calibration The basic principle, that losses in the MgB2 sample can be determined from calibration using a heater wound together with the sample, was veriﬁed at 42 K (just above the critical temperature of MgB2). The temperature increase was measured ﬁrst when passing a DC current in the heater, and then when passing a DC current in the MgB2 sample. In both cases the current and the voltage drop was recorded. In Fig. 5 the temperature response is given as function of input power with durations of 5 s and 20 s. The response is virtually independent of whether the heat is generated in the heater or the MgB2 sample. Calibration is performed to determine the function (4). A typical response of the copper thermometer is shown in Fig. 6. From such
3.6. Current injection When injecting transport current into the sample, the heat transfer through the current leads should be limited. In the system, the current leads consist of three parts. (1) Copper feed-throughs 10 mm 10 mm, immersed in liquid nitrogen on the outside of the cryostat. (2) BSCCO/Ag conductors soldered to the copper feed-throughs inside the cryostat. The number of parallel BSSCO/ Ag tapes depends on the maximum desired transport current in the sample. The length of the tapes is about 0.5 m (half a turn in the evacuated space below the sample holder). (3) The MgB2 sample wire is soldered to the BSCCO/Ag tape over a length of about 100 mm, and the entire joint is thermally anchored to a copper plate in direct contact with the cold head. The MgB2 sample wire makes a half turn around the sample holder (0.5 m) before entering the top of the sample holder and ﬁnally the 0.4 m long measurement area on the opposite side of the sample holder. The long distances are chosen to reduce heat transport through the current leads and to avoid any inﬂuence of losses in e.g. the BSCCO/Ag conductors. It is important that the MgB2 sample wire is at the highest temperature in the section where the AC losses are measured. Otherwise, for transport currents close to the critical current, the wire may go normal. As described in Section 3.3, a heater at the top of the sample holder raises the temperature in this area compared to the cold head temperature. Hence, the MgB2 sample wire temperature increases as it enters the top of the sample holder. However, at the half turn (0.4 m) long measuring area on the opposite side, the temperature is practically uniform.
Fig. 5. Comparison of temperature response at 42 K between power dissipated in the heater and in the MgB2 sample.
Fig. 6. Response of copper thermometer during calibration at 33.5 K. The preperformed calibration of the copper thermometer with a Cernox thermometer shows that the resistance increase of 0.93 mX corresponds to a temperature increase of 0.53 K.
H. Taxt et al. / Cryogenics 54 (2013) 44–49
a curve, the temperature increase for different durations can be extracted and calibration curves as in Fig. 7 can be drawn. When calibration is performed at different temperatures, these curves determine the expression (4). 4.2. Measured AC losses AC loss measurements have been performed on a tape-shaped multi-ﬁlamentary MgB2 superconductor manufactured by Columbus Superconductors. The cross-sectional area of the sample is 0.95 mm 4.2 mm, of which the MgB2 ﬁlaments constitute 18%. Niobium serves as a barrier around each ﬁlament and the sheath material is non-magnetic cupronickel (70/30). The self-ﬁeld critical current is about 260 A at the measurement temperature 33.5 K. The ﬁlaments are not twisted. The measurement results are given in Fig. 8. The frequency is 50 Hz and the magnetic ﬁeld applied in parallel with the tape face. Losses are measured as function of current with no externally applied ﬁeld, and as function of current combined with a magnetic ﬁeld of 36 mTpeak. The magnetic ﬁeld and transport current are in-phase with each other. In addition losses due to applied ﬁeld only (up to 100 mT) are shown at the vertical axis. The relatively low magnetic ﬁelds used are a consequence of the loss level in the sample (as expected from a broad non-twisted DC wire).
The MgB2 superconductor is, like the BSCCO/Ag superconductor, built up of a number of ﬁlaments in a metal matrix. It is reasonable to believe that the two superconductors behave in a similar way. In Fig. 8 the dashed lines corresponds to the Norris strip and ellipse equations , commonly used for BSCCO/Ag conductors in selfﬁeld. The measured losses tend to move from the strip equation towards the ellipse equation at higher currents, as observed in some studies of BSCCO/Ag conductors [14,15]. For the combined ﬁeld and transport current, the losses are compared to the Carr equations  using an effective area  of the ﬁlament region of 3.2 mm2 and a full penetration ﬁeld of 67 mT, both obtained from . Quantitatively, the AC losses follow the same pattern as expected from the theory of fully coupled ﬁlaments, which was used for non-twisted BSCCO/Ag conductors. 5. Conclusions The presented calorimetric AC loss measurement system gives reliable results and can be a valuable tool in the development of AC optimized MgB2 superconductors. Beneﬁts of the system are the reliability and the wide range of magnetic ﬁelds and transport currents attainable. Furthermore, if and when MgB2 superconductors with loss levels acceptable for AC applications appear, the system can be used in the design phase of MgB2 based AC power components. The ﬁrst results obtained with the system indicate a similar behavior of the MgB2 multi-ﬁlamentary tape as for the BSCCO/Ag tape. Acknowledgement This work has been supported in part by the Nowitech programme and by the Research council of Norway. References
Fig. 7. Calibration curves for three different temperatures.
Fig. 8. Measured AC losses as function of transport current with no externally applied magnetic ﬁeld (lower curve) and with an externally applied magnetic ﬁeld of 36 mTpeak (upper curve). At the vertical axis losses with no transport current are given. The lines represent modeled values.
 Malagoli A, Bernini C, Braccini V, Fanciulli C, Romano G, Vignolo M. Fabrication and superconducting properties of multiﬁlamentary MgB2 conductors for AC purposes: twisted tapes and wires with very thin ﬁlaments. Supercond Sci Technol 2009;22:1–6.  Ashworth SP, Suenaga M. Measurement of ac losses in superconductors due to ac transport currents in applied ac magnetic ﬁelds. Physica C 1999;313: 175–87.  Rabbers JJ, ten Haken B, ten Kate HHJ. Measuring transport current loss of BSCCO/Ag tapes exposed to external AC magnetic ﬁeld. Physica C 1998; 310:101–5.  Magnusson N, Hörnfeldt S. Calorimetric apparatus for alternating current loss measurement on high-temperature superconductors. Rev Sci Instrum 1998;69:3320–5.  See KW, Cook CD, Dou SX. Innovative calorimetric AC loss measurement of HTSC for power applications. IEEE Trans Appl Supercond 2011;21:3261–4.  Ashworth SP, Suenaga M. The calorimetric measurement of losses in HTS tapes due to ac magnetic ﬁelds and transport currents. Physica C 1999;315:79–84.  Magnusson N, Hörnfeldt S, Rabbers JJ, ten Haken B, ten Kate HHJ. Comparison between calorimetric and electromagnetic total ac loss measurement results on a BSCCO/Ag tape. Supercond Sci Technol 2000;13:291–4.  Rostila L, Demencˇík E, Šouc J, Brisigotti S, Kovácˇ P, Polak M, et al. Magnesium diboride wires with nonmagnetic matrices – AC loss measurement and numerical calculations. IEEE Trans Appl Supercond 2011;21:3338–41.  Young EA, Bianchetti M, Grasso G, Yang Y. Characteristics of AC loss in multiﬁlamentary MgB2 tapes. IEEE Trans Appl Supercond 2007;17:2945–8.  See KW, Xu X, Horvat J, Cook CD, Dou SX. Calorimetric AC loss measurement of MgB2 superconducting tape in an alternating transport current and direct magnetic ﬁeld. Supercond Sci Technol 2012;25:115016.  Magnusson N, Schönborg N, Wolfbrandt A, Hörnfeldt S. Improved experimental set-up for calorimetric AC loss measurement on HTSs carrying transport current in applied magnetic ﬁelds at variable temperatures. Physica C 2001;354:197–201.  Taxt H, Magnusson N, Runde M, Brisigotti S. AC loss measurements on MgB2 superconductors with non-magnetic sheath material. IEEE Trans Appl Supercond 2013;23:8200204.  Norris WT. Calculation of hysteresis losses in hard superconductors carrying ac: isolated conductors and edges of thin sheets. J Phys D 1970;3:489–507.  Fukunaga T, Oota A. AC transport losses under self ﬁelds in Ag-sheathed (Bi, Pb)2Sr2Ca2Cu3Ox conductors. Physica C 1997;291:201–6.
H. Taxt et al. / Cryogenics 54 (2013) 44–49  Gherardi L, Bettinelli D, Spreaﬁco S, Gömöry F. Estimation of Jc(B) dependence from self-ﬁeld alternating current (AC) losses measured on Bi-2223/Ag tapes. Physica C 1998;310:52–6.  Carr WJ. AC losses from the combined action of transport current and applied magnetic ﬁeld. IEEE Trans Magn 1979;15:240–3.
 Magnusson N. Semi-empirical model of the losses in HTS tapes carrying AC currents in AC magnetic ﬁelds applied parallel to the tape face. Physica C 2001;349:225–34.